Field emission enhancement of Au-Si nano-particle-decorated silicon nanowires
© Zhao et al; licensee Springer. 2011
Received: 30 May 2010
Accepted: 25 February 2011
Published: 25 February 2011
Au-Si nano-particle-decorated silicon nanowire arrays have been fabricated by Au film deposition on silicon nanowire array substrates and then post-thermal annealing under hydrogen atmosphere. Field emission measurements illustrated that the turn-on fields of the non-annealed Au-coated SiNWs were 6.02 to 7.51 V/μm, higher than that of the as-grown silicon nanowires, which is about 5.01 V/μm. Meanwhile, after being annealed above 650°C, Au-Si nano-particles were synthesized on the top surface of the silicon nanowire arrays and the one-dimensional Au-Si nano-particle-decorated SiNWs had a much lower turn-on field, 1.95 V/μm. The results demonstrated that annealed composite silicon nanowire array-based electron field emitters may have great advantages over many other emitters.
Silicon is one of the most promising candidates and plays a significant role in the micro-electronic field. One-dimensional silicon nanowires (SiNWs) have been fabricated by many approaches, such as chemical vapor deposition , laser ablation , thermal evaporation , chemical etching [4, 5] methods, etc., since they were first fabricated via the vapor-liquid-solid (VLS) mechanism . Among the above mentioned methods, for dealing with the challenges that the nanowires should grow aligned in the same direction with high purity, chemical etching method is a simple and convenient way to fabricate pure well-aligned SiNWs.
Fabrication of electron-emitting nano-materials [7–9] and application of electron field emitters on the flat panel displays  have attracted much attention on the studies of one-dimensional materials because of their advantages of high aspect ratio, stable structure, and high electron field emission (FE) properties. In the studied field emitters [11–16], SiNW-based emitters [17–21] have been widely studied. In order to improve the FE property, various kinds of modification have been done on SiNWs, such as H2 plasma surface treatment of Si nanowires [22, 23], Mo-modified Si field emitter , Ni-implanted Si samples , and IrO2 coated on silicon nanotips . Gold is a metal with low resistivity and high structure stability. However, the influence of Au coating and post-annealing treatment on FE properties of silicon nano-structures has not been reported. In this article, the influence of Au coating and post-annealing treatment on FE properties of SiNWs and the enhancement of FE property by modifying as-grown SiNWs to Au nano-particles-decorated SiNWs have been investigated.
A simple chemical approach was utilized here to synthesize SiNWs . In this procedure, n-type 〈100〉 silicon wafer was used as substrate and ultrasonically cleaned in acetone and ethanol for 5 to 10 min followed by washing in de-ionized water. The cleaned substrates were immersed in AgNO3/HF solution to deposit Ag catalyst for 1 min, where the concentrations of AgNO3 and HF were 0.01 mol/l and 8%, respectively. Afterward, they were quickly transferred into H2O2/HF solution to fabricate SiNWs at room temperature, where the concentrations of H2O2 and HF were 0.6 and 8%, respectively. After 1-h chemical etching, the color of silicon surface became dark, which indicated the formation of SiNWs. The as-grown SiNWs were post-treated in 1% diluted HF solution to remove the SiO2 layers coated outside. Au film deposition was carried out by using DC magnetron sputtering technology in Ar atmosphere (1 Pa), and the sputtering current was 20 mA. The thicknesses of the Au films were nominally defined as 20, 60, and 80 nm for different deposition times. Further experiments were done by annealing the SiNWs with Au films at 500, 650, and 800°C, respectively, in a quartz tube furnace and H2 atmosphere for 2 h.
The morphology and structure characterization of the nanowires were done by scanning electron microscope (SEM) (S-4800, Hitachi) and transmission electron microscope (TEM) (FEI TECNAI F30, Philips). FE measurements were carried out in the high vacuum chamber with a base pressure of 3 × 10-7 Pa. The distance between cathode and anode was indicated by an electronic digital display indicator and could be adjusted in a scale of 0 to 5 cm. Applied voltages up to 10 kV could be impressed on the flat anode to ensure that the emission current could be tested and detected with a digital multimeter.
Result and discussion
Figure 1b shows TEM image of the 650°C post-annealed Au20/SiNWs. From Figure 1b, it can be seen that Au20/SiNWs are about 120 nm in diameter, and there are many nano-sized particles with the size ranging from 10 to 48 nm being dispersively distributed along the axis of the post-annealed Au20/SiNW. The inset of HRTEM image in Figure 1b illustrates that nano-sized particles on the surface of the post-annealed Au/SiNWs are nano-crystalline particles. The interplanar spacing calculated from HRTEM image of the nanoparticle is approximately 0.26 nm, which can be attributed to the  planes of Au2Si phase . Compared with as-grown SiNWs , the morphology of the post-annealed Au20/SiNW has not been changed much and still shows the wire-shape in which many Au nano-particles covered on the surface of nanowire. These observations indicate that Au-Si nano-particle decorated SiNWs can be fabricated during annealing at a high temperature.
FE parameters of Au film-coated SiNWs with different thicknesses
E on, (V/μm)
E J = 100 μA/cm2(V/μm)
where β is the field enhancement factor, A and B are constants equal to 1.54 × 10-6 A eV V-2 and 6.83 × 103 eV-3/2 V μm-1, respectively. Thus, β or Φ could be calculated via the slope of the straight line of ln(J/E 2) and 1/E. Because the area of SiNW array is large and the morphology is relatively uniform, little change of the morphology has been made after Au deposition. The authors have the evidence to assume that the value of β is approximately equal to each other, and so Φ will change for different emitters. According to the F-N plots given in the inset of Figure 2, Φ can be calculated to be 4.15, 4.29, 4.51, and 4.98 eV for as-grown SiNWs, Au20/SiNWs, Au60/SiNWs, and Au80/SiNWs, respectively, as shown in Table 1. FE property of the emitter is highly dependent on their composition, tip sharpness, aspect ratio, conductivity, and work function. High Φ makes electron FE difficult and reduces FE property of the emitter. These observations further confirm that Au deposition without annealing is not effective in the improvement of FE property.
FE parameters of Au20/SiNWs before and after post-annealing at different temperatures
E on (V/μm)
E J = 200 μA/cm2(V/μm)
The FE properties of emitters are related with their composition, tip sharpness, aspect ratio, conductivity, and work function. Au has a high work function (Φ), i.e. 5.55 eV , which is larger than that of Si (about 4.15 eV ). When continuous Au layer covered on SiNWs, electron FE comes from the Au tip covered on SiNWs and not from the tip of SiNWs. High work function of the emitter makes electron emission difficult and reduces more the FE property of the emitter. Therefore, E on values of the Au/SiNWs are higher than that of the as-grown SiNWs, and the FE properties of the Au/SiNWs are worse than that of as-grown SiNWs. However, the post-annealing processing above 650°C for the Au/SiNWs makes the J-E curves move to lower applied field, and lower E on values, which is in the range from 1.95 to 2.35 eV, can be obtained. Those prove that the FE properties of Au/SiNWs can be remarkably enhanced by the post-annealing processing above 650°C. TEM and HRTEM images in Figure 1 illustrate that Au-Si nano-particles had been formed at the surface of Au20/SiNWs after post-annealing at 650°C, and that the Au-Si nano-particle-decorated SiNWs had been fabricated. Previous studies show that gold silicide, such as Au2Si [31, 32] and AumSin , have been observed, and some kind of composition has good optical, excellent electron transportation, and FE properties. For the Au2Si nano-particle-decorated SiNWs, electrons transport near and on the surface of the composite region. Tunneling effect happens when the energy states are distributed in the band gap and the electrons in the conduction band of the SiNWs can be tunneled . This will make the surface potential barrier height of the emitter to be reduced. On the other hand, the similar enhancement results, in which the differences are very small, have been observed in SiNWs coated by Au film with different thicknesses and then post-annealed at 650°C. It is due to the formation of similar micro-structures of the Au-Si nano-particle-decorated SiNWs. Thus, we have the evidence to believe that uniform Au-Si nano-particle-decorated SiNWs could improve the FE properties of SiNWs by enhancing electron transportation and reducing surface potential barrier height of emitter.
Au film coating on the tip of SiNWs reduces the FE properties of SiNWs because of Au having high work function. Well-aligned Au-Si nano-particle-decorated SiNW arrays have been fabricated by Au film deposition and post-annealing above 650°C, which have excellent FE properties. The lowest E on value of the Au-Si nano-particle-decorated SiNWs is about 1.95 V/μm, and J can reach 200 μA/cm2 at the applied field of 2.79 V/μm. Improvement of the FE properties may be due to Au-Si nano-particle decoration on the top surface of SiNWs, which enhances electron transportation in the SiNWs and reduces the surface potential barrier height of the emitter. These results indicate that the post-annealed Au/SiNW arrays would be used in the field of flat panel displays in the future.
scanning electron microscope
transmission electron microscope
The authors gratefully acknowledge the financial support of the National Basic Research Program of China (Grant No: 2010CB832905) and the partial support provided by the Key Project of the Chinese Ministry of Education (Grant No. 108124).
- Liu ZQ, Pan ZW, Sun LF, Tang DS, Zhou WY, Qian LX, Xie SS: Synthesis of silicon nanowires using AuPd nanoparticles catalyst on silicon substrate. J Phys Chem Solids 2000, 61: 1171. 10.1016/S0022-3697(99)00380-7View ArticleGoogle Scholar
- Morales AM, Lieber CM: A Laser Ablation Method for the Synthesis of Crystalline Semiconductor Nanowires. Science 1998, 279: 208. 10.1126/science.279.5348.208View ArticleGoogle Scholar
- Feng SQ, Yu DP, Zhang HZ, Bai ZG, Ding Y: The growth mechanism of silicon nanowires and their quantum confinement effect. J Crys Growth 2000, 209: 513. 10.1016/S0022-0248(99)00608-9View ArticleGoogle Scholar
- Peng KQ, Huang ZP, Zhu J: Fabrication of large-area silicon nanowire p-n junction diode arrays. Adv Mater 2004, 16: 73. 10.1002/adma.200306185View ArticleGoogle Scholar
- Zhao F, Cheng GA, Zheng RT, Xia LY: E_ect of the Microstructure of Ag Catalysts in the Fabricating Process of Silicon Nanowires. J Korean Phys Soc 2008, 52: S104-S107. 10.3938/jkps.52.104View ArticleGoogle Scholar
- Wanger RS, Ellis WC: Vapor-Liquid-Solid Mechanism of Single Crystal Growth. Appl Phys Lett 1964, 4: 89. 10.1063/1.1753975View ArticleGoogle Scholar
- Iijima S: Helical microtubules of graphitic carbon. Nature 1991, 354: 56. 10.1038/354056a0View ArticleGoogle Scholar
- Rinzler AG, Hafner JH, NIkolaev P, Nordlander P, Colbert DT, Smalley RE, Lou L, Kim SG, Tománe kD: Unraveling Nanotubes: Field Emission from an Atomic Wire. Science 1995, 269: 1550–1553. 10.1126/science.269.5230.1550View ArticleGoogle Scholar
- Chen KF, Deng JH, Zhao F, Cheng GA, Zheng RT: Influence of Zn ion implantation on structures and field emission properties of multi-walled carbon nanotube arrays. Sci China Technol Sci 2010, 53: 776–781. 10.1007/s11431-009-0384-xView ArticleGoogle Scholar
- Lee NS, Chung DS, Han IT, Kang JH, Choi YS, Kim HY, Park SH, Jin YW, Yi WK, Yun MJ, Jung JE, Lee CJ, You JH, Jo SH, Lee CG, Kim JM: Application of carbon nanotubes to field emission displays. Diam Relat Mater 2001, 10: 265. 10.1016/S0925-9635(00)00478-7View ArticleGoogle Scholar
- Park CJ, Choi DK, Yoo J, Yi GC, Lee CJ: Enhanced field emission properties from well-aligned zinc oxide nanoneedles grown on the Au/Ti/n-Si substrate. Appl Phys Lett 2007, 90: 083107. 10.1063/1.2643979View ArticleGoogle Scholar
- Zhu YW, Zhang HZ, Sun XC, Feng SQ, Xu J, Zhao Q, Xiang B, Wang RM, Yu DP: Efficient field emission from ZnO nanoneedle arrays. Appl Phys Lett 2003, 83: 144. 10.1063/1.1589166View ArticleGoogle Scholar
- Xiang B, Zhang Y, Wang Z, Luo XH, Zhu YW, Zhang HZ, Yu DP: Field-emission properties of TiO2 nanowire arrays. J Phys D 2005, 38: 1152. 10.1088/0022-3727/38/8/009View ArticleGoogle Scholar
- Wu ZS, Deng SZ, Xu NS, Chen J, Zhou J, Chen J: Needle-shaped silicon carbide nanowires: Synthesis and field electron emission properties. Appl Phys Lett 2002, 80: 3829. 10.1063/1.1476703View ArticleGoogle Scholar
- Zhou J, Xu NS, Deng SZ, Chen J, She JC, Wang ZL: Large-area nanowire arrays of molybdenum and molybdenum oxides: synthesis and field emission properties. Adv Mater 2003, 15: 1835. 10.1002/adma.200305528View ArticleGoogle Scholar
- Chen J, Deng SZ, Xu NS, Wang SH, Wen XG, Yang SH, Yang CL, Wang JN, Ge WK: Field emission from crystalline copper sulphide nanowire arrays. Appl Phys Lett 2002, 80: 3620. 10.1063/1.1478149View ArticleGoogle Scholar
- Wong WK, Meng FY, Li Q, Au FCK, Bello I, Lee ST: Field-emission properties of multihead silicon cone arrays coated with cesium. Appl Phys Lett 2002, 80: 877. 10.1063/1.1446990View ArticleGoogle Scholar
- Huang CT, Hsin CL, Huang KW, Lee CY, Yeh PH, Chen US, Chen LJ: Er-doped silicon nanowires with 1.54 mu m light-emitting and enhanced electrical and field emission properties. Appl Phys Lett 2007, 91: 093133. 10.1063/1.2777181View ArticleGoogle Scholar
- Kulkarni NN, Bae J, Shih CK, Stanley SK, Coffee SS, Ekerdt JG: Low-threshold field emission from cesiated silicon nanowires. Appl Phys Lett 2005, 87: 213115. 10.1063/1.2136217View ArticleGoogle Scholar
- Tang YH, Sun XH, Au FCK, Liao LS, Peng HY, Lee CS, Lee ST, Sham TK: Microstructure and field-emission characteristics of boron-doped Si nanoparticle chains. Appl Phys Lett 2001, 79: 1673. 10.1063/1.1396313View ArticleGoogle Scholar
- Zhao F, Zhao DD, Wu SL, Cheng GA, Zheng RT: Fabrication and Electron Field Emission of Silicon Nanowires Synthesized by Chemical Etching. J Korean Phys Soc 2009, 55: 2681. 10.3938/jkps.55.2681View ArticleGoogle Scholar
- Au FCK, Wong KW, Tang YH, Zhang YF, Bello I, Lee ST: Electron field emission from silicon nanowires. Appl Phys Lett 1999, 75: 1700. 10.1063/1.124794View ArticleGoogle Scholar
- Jo SH, Lao JY, Ren ZF, Farrer RA, Baldacchini T, Fourlcas JT: Field-emission studies on thin films of zinc oxide nanowires. Appl Phys Lett 2003, 83: 4821. 10.1063/1.1631735View ArticleGoogle Scholar
- Ha JK, Chung BH, Han SY, Choi JO: Drastic changes in the field emission characteristics of a Mo-tip field emitter array having PH3-doped a-Si: H as a resistive layer material throughout vacuum packaging processes in'a field emission display. J Vac Sci Technol B 2002, 20: 2080. 10.1116/1.1508817View ArticleGoogle Scholar
- Ok YW, Seong TY, Choi CJ, Tu KN: Field emission from Ni-disilicide nanorods formed by using implantation of Ni in Si coupled with laser annealing. Appl Phys Lett 2006, 88: 043106. 10.1063/1.2167797View ArticleGoogle Scholar
- Chen TM, Hung JY, Pan FM, Chang L, Wu SC, Tien TC: Pulse Electrodeposition of Iridium Oxide on Silicon Nanotips for Field Emission study. J Nanosci Nanotechnol 2009, 9: 3264. 10.1166/jnn.2009.203View ArticleGoogle Scholar
- Joint Committee on Powder Diffraction Standards (JCPDS) card number 40–1140
- Fowler RH, Nordheim L: Electro emission in intense electric fields. Proc. R. Soc. Lond. Ser. A 1928, 119: 173. 10.1098/rspa.1928.0091View ArticleGoogle Scholar
- Hasegawa Y, Jia JF, Inoue K, Sakai A, Sakurai T: Elemental contrast of local work function studied by scanning tunneling microscopy. Surf Sci 1997, 386: 328. 10.1016/S0039-6028(97)00332-4View ArticleGoogle Scholar
- Zhang TH, Wu YG: Science and Application of Ion Beam Materials Modification. Beijing: Science Press of Beijing; 1999.Google Scholar
- Wu JS, Dhara S, Wu CT, Chen KH, Chen YF, Chen LC: Growth and optical properties of self-organized AU(2)Si nanospheres pea-podded in a silicon oxide nanowire. Adv Mater 2002, 14: 1847. 10.1002/adma.200290017View ArticleGoogle Scholar
- Zhirnov VV, Bormatova L, Givargizov EI, Plekhanov PS, Son UT, Galdetsky AV, Belyavsky BA: Field emission properties of Au---Si eutectic. Appl Surf Sci 1996, 94/95: 144. 10.1016/0169-4332(95)00362-2View ArticleGoogle Scholar
- Compagnini G, Urso LD, Cataliotti RS, Puglisi O, Scandurra A, La Fata P: Properties of Au/Si nanostructured films obtained by jet-cooled cluster beam deposition. J Phys Chem C 2007, 111: 7251. 10.1021/jp0684877View ArticleGoogle Scholar
- Wan Q, Wang TH, Lin CL: Self-assembled Au-Si alloy nanocones: synthesis and electron field emission characteristics. Appl Surf Sci 2004, 221: 38. 10.1016/S0169-4332(03)00953-XView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.